- Open Access
Superhydrophilic self-cleaning surfaces based on TiO2 and TiO2/SiO2 composite films for photovoltaic module cover glass
© Jesus et al.; licensee Springer. 2015
- Received: 21 November 2014
- Accepted: 16 February 2015
- Published: 12 March 2015
Self-cleaning surfaces have excelled in recent years in energy and environmental fields. In particular, in solar energy area, these surfaces are used to avoid soiling accumulation on photovoltaic (PV) modules. So far TiO2 has been widely used due to its photocatalytic activity and photo-induced superhydrophilicity. However, this oxide has some limitations since it reduces the glass transmittance and it rapidly reestablish the water contact angle in dark environments. In order to circumvent these limitations, composites TiO2/SiO2 have been proposed. For photovoltaic application, besides a good transparency in the wavelength region 300–1800 nm and self-cleaning properties, the coating should also present long durability and adequate adhesion to endure the outdoor conditions. Aiming at developing a coating with these properties, in this work, TiO2/SiO2 composites containing different titanium content have been synthesized and compared with pure TiO2 films in relation to adhesion, transparency and hydrophilicity. Both films have been deposited over low iron float glass substrates by sol–gel dip-coating technique and different calcination temperatures (400, 500, 600°C) and Si/Ti molar rates (Si86Ti14, Si40Ti60) have been considered. TiO2/SiO2 films showed higher transmittance in visible range compared with pure TiO2. TiO2/SiO2 films showed superhydrophilic character before and after ultraviolet irradiation, with water contact angles near to 0°. Furthermore, as predicted, TiO2/SiO2 films could keep the superhydrophilic character in dark environments, in contrast with pure TiO2 films. Both TiO2 and TiO2/SiO2 films exhibited good adherence and it is shown that higher calcination temperatures and higher titanium content enhance such property. All films presented abrasion resistant property in contact with sponge and detergent. It has been demonstrated that high transmittance, self-cleaning and adherent composite has been obtained by a simple sol–gel route presenting good potential to be applied on photovoltaics systems.
- TiO2/SiO2 composite
- Thin film
- Self-cleaning surfaces
TiO2 is widely used as a photocatalyst and it can be applied in environmental and energy fields, including self-cleaning surfaces, air and water purification systems, anti-fogging surfaces, among others . The self-cleaning property of TiO2 is provided by two photo-induced phenomena . The first one is the photocatalysis, wherein organic contaminants adsorbed on film surface are decomposed under ultraviolet light . This property allows TiO2 to be applied in air and water purification systems as well as for self-cleaning surfaces. The second one is the photo-induced superhydrophilicity, wherein contaminants and dirt are washed off the surface by the film of water on it . On the superhydrophilic surface, a very small water contact angle is formed (θ ≤ 5°), as the water tends to spread completely across the surface rather than forming droplets. This makes the surface anti-fogging and easy- washing [1,3]. Commercial self-cleaning and anti-fogging surfaces are usually made of TiO2 thin films . However, TiO2 thin films have some limitations, for example, they reduce the glass transmittance due to the high refractive index of TiO2 . Moreover, in dark environments TiO2 films have a rapid reestablishment of hydrophobicity, which affects negatively the self-cleaning efficiency . TiO2/SiO2 composite films can circumvent these limitations, slowing down the increase of water contact angle in dark environments and presenting higher transmittance with respect TiO2, which is essential for the application as a self-cleaning surface in solar energy area [2,6,7]. Self-cleaning surface are indeed important for PV application, since the dust, pollution, and other particles accumulation reduce the transparency of the PV module cover glasses and consequently decrease the electrical performances of the modules. In particular for CPV modules, the soling effect is particularly severe, since such modules mainly collect the sun direct light which can be strongly reduced by the dust accumulation on the module. Performance degradation up to 30% has been measured . Several studies have been made to address the severity of deposited particles (like dust, water stains, carbon from smoke, and pollen from agricultural regions) on the efficiency reduction of solar devices, which results in additional costs either from oversizing the system or from cleaning them . For photovoltaic application, besides the self-cleaning properties, the coating should present adequate adhesion and transparency in the wavelength region 300–1800 nm. Several techniques have been reported for the deposition of TiO2 and SiO2 thin films, like CVD , sputtering [11-13], electron beam evaporation  and sol–gel process [2,6,7,15]. Sol–gel method has the advantage of offering small and large area deposition at a low cost . In literature, however, detailed analyses of the anti-soling film in term of structural properties, transparency, robustness and cost are still missing. In this work, pure TiO2 and TiO2/SiO2 composite films containing different titanium content have been deposited over glass substrates by sol–gel dip-coating method aiming at obtaining super hydrophilic, adherent and transparent coating. The influence of the titanium content and the calcination temperature has been evaluated. The coatings have been compared and characterized regarding their optical, mechanical and microstructural properties.
Thin film deposition
Low iron float glass (LIFG) substrates 4 mm thick(Pilkington Optiwhite Low Iron) were ultrasonically cleaned with ethanol (EtOH) and air dried. Titanium isopropoxide (TIPT), tetraethyl orthosilicate (TEOS) and isopropanol (IspOH) (99%w/w) were used as precursors and solvent for sol gel solution. TiO2/SiO2 composite films were prepared with different Si/Ti molar rate mixed solutions. The abbreviation Si86Ti14, Si40Ti60 is used to express the Si/Ti molar rate mixed solutions used to prepare the composite composed by the mixture of SiO2 and TiO2 oxides. TIPT:IspOH:H2O molar ratio was 1:97:0,5 and TEOS:IspOH:H2O molar ratio was 1:47:2. Film deposition was performed using the dip-coating equipment Marconi (MA 765) at room conditions (20°C, relative air humidity lower than 30%). LIFG substrates were immersed and emerged with a speed of 3,6 mm/s. Then, films were treated in muffle furnace at 400, 500 and 600°C for 2 hrs under air.
Light transmittance (T) of the samples was measured by JASCO V-670 spectrophotometer in the range of 200–2100 nm. Surface hydrophilicity was evaluated by water contact angle (WCA) measurements using a KRUSS DS100 goniometer connected to a video camera at room temperature (25°C, relative air humidity lower than 50%). For these measurements, deionised water droplets volume was fixed at 2 μL, 2 drops per sample and 3 replicates were used. WCA measurements were performed before and after ultraviolet (UV) light irradiation (15 W mercury lamp–Techlux emitting 254 nm wavelength).The samples were exposed to light irradiation, 5 cm far from the light source. Adherence was evaluated by measuring the critical load in the point where the first coating delamination occurs. Load application and scratch formation were performed by VTT Tech Scratch Tester equipment. Scratch test parameters were: translation speed:10 mm/min, loading speed: 100 N/min, initial load: 0-1 N and final load: 40 N. Abrasion test was performed in a tribometer Biceri equipment. Abrasion test was carried out between a mobile probe fixed in a carriage with reciprocal movement and a fixed pin. The pin was manufactured by gluing a piece of 50 x 50 mm yellow part of a Scotch Brites ponge on a standard pin. Before testing, the sponge was lubricated with commercial diluted detergent (MISTOL 66% + 33% distilled water). Test time was 7 hrs, corresponding to 25.000 cycles of movement of the mobile surface. All the mechanical tests were carried out at room conditions (25°C, 30% relative air humidity). After abrasion test the light transmittances was measured. The film thickness and microstructure was evaluated by surface imaging and RMS roughness measurements using an atomic force microscope (AFM) Asylum Research - MFP-3D in tapping mode. RMS roughness values were calculated by spectral analysis on 1 μm2 areas. This analysis have been carried out at room conditions (20°C, 20% relative air humidity) using C160TS-R3 probe (silicon, elastic constant = 26 N/m) and the software MFP3D (version 13). Raman spectra were collected on a Horiba JobinYvon LABRAM-HR 800 spectrograph, equipped with a 633 nm helium-neon laser, 20 mW of power, attached to an Olympus BHX microscope equipped with 10, 50, and 100X lenses.
TiO2/SiO2 composite films showed high %T (>85%) in visible-NIR range, which is fundamental for solar energy application . Si86Ti14 composite film treated 400°C and 500°C presented the best result of %T with value ~ 1% lower compared to the uncoated glass. Whereas, both samples, Si40Ti60 composite and TiO2 treated at 400°C presented a transmittance of 6% and 11% lower than the uncoated glass respectively. It is possible to notice that all composite samples show an improvement in transmittance compared to pure TiO2 films. It is possible also to assess (Figure 1) the effect of the calcination temperature on the thin film transmittance. For all the coatings, higher temperature resulted in lower %T due to the densification of the coatings and to the increase of the refractive index value . While titanium content increases, %T of the thin film decreases. This can be explained by the fact that TiO2 has higher refractive index (RI) (n ≈ 2,5) than SiO2 (n ≈ 1,45). Consequently, higher RI results in lower %T of the coatings .
Water contact angles before and after ultraviolet irradiation for 30 minutes
TiO 2 400°C
TiO 2 500°C
TiO 2 600°C
Si 86 Ti 14 400°C
Si 40 Ti 60 400°C
Before UV ( 0 )
(30,0 ± 0,2)
(27,0 ± 0,2)
(26,0 ± 0,2)
(6,0 ± 0,1)
(6,0 ± 0,1)
After UV ( 0 )
(6,0 ± 0,2)
(4,0 ± 0,2)
(4,0 ± 0,2)
(1,0 ± 0,1)
(0,1 ± 0,1)
Si 86 Ti 14 500°C
Si 40 Ti 60 500°C
Si 86 Ti 14 600°C
Si 40 Ti 60 600°C
Before UV ( 0 )
(1,0 ± 0,1)
(1,0 ± 0,1)
(1,0 ± 0,1)
(1,0 ± 0,1)
(32,0 ± 0,2)
After UV ( 0 )
(0,1 ± 0,1)
(0,1 ± 0,1)
(0,1 ± 0,1)
(0,1 ± 0,1)
(30,0 ± 0,2)
AFM analysis revealed that the composite thin film treated at 400°C is more porous than pure TiO2 (Figure 3). Figure 3-A presents a typical morphology of TiO2 400°C, crystalline with particle size = 6,2 nm. Figure 3-B shows clearly that TiO2/SiO2 film presents a sponge-like morphology with rather large cavities which indicates an important surface porosity. Houmard et al.(2007) has shown similar morphology when it was prepared a TiO2/SiO2 composite by using a different sol composition and sol–gel spin-coating process . The composite film shown in Figure 3-B is rougher (RMS = 2,7 nm) than TiO2 film (RMS = 1,4 nm) in Figure 3-A, due to this morphology. The formation of this microstructure (Figure 3-B) is not yet completely understood, but it is speculated that modifications in the structure of –(O–Si)n– polymeric chains fixed on TiO2 crystallites, which arise from modifications in the silica sol formulations, can lead to variations in the morphological properties of composite films . The average thickness of the coating, measured by AFM in five points of the sample, has been estimated as 63 nm for Si40Ti60, 85 nm for Si86Ti14 and 45,5 nm for TiO2.
All TiO2 and TiO2/SiO2 films have maintained transmittance after 25000 cycles in abrasion test, showing how these films would not be affected or scratched in a conventional cleaning process. These results corroborate with adherence results, showing how these films are well adhered to the substrate, and can support an abrasion procedure, like the one produced by cleaning. It is well known that wear is closely related to the adhesion of thin film to the substrates. If the film adherence is poor, the film will wear off quickly. If the film adherence is good, the film will resist to wear. Therefore, TiO2 and TiO2/SiO2 films have exhibited good mechanical properties which are required for long durability in outdoor applications.
TiO2/SiO2 high transmittance, self-cleaning, abrasion resistant and adherent films were obtained by a simple sol–gel route. 500°C treated films showed better mechanical property with respect to 400°C treated films and better optical property with respect 600°C treated films. TiO2/SiO2 composite film presented an important surface porosity which is rougher than TiO2 film. TiO2/SiO2 composite films presented higher transmittance, lower water contact angle and similar adherence/abrasive resistance compared to pure TiO2 films. These properties are essential for application as a self-cleaning surface in solar energy area, when transparency and low water contact angles are required. TiO2 and TiO2/SiO2 films have presented good mechanical properties which are required for outdoor applications and necessary to resist in harsh environmental conditions.
I would thank CEFET-MG, CNPq for financial support, INCT-Acqua for Raman analyses support. The research has been partially supported by the Commission under the Grant Agreement N.295303 Sun on Clean Project, in the IRSES Seventh Framework Program.
- Nakata K, Fujishima A (2012) TiO2 photocatalysis: Design and applications. J Photochem Photobiol C 13:169–189View ArticleGoogle Scholar
- Guan K (2005) Relationship between photocatalytic activity, hydrophilicity and self-cleaning effect of TiO2/SiO2 films. Surface Coatings Technol 191:155–160View ArticleGoogle Scholar
- Fujishima A, Tryk DAZX (2008) TiO2 photocatalysis and related surface phenomena. Surf Sci Rep 63:515–582View ArticleGoogle Scholar
- Wang R, Hashimoto K, Fujishima A, Chikuni M, Kojima E, Kitamura A, Shimohigoshi M, Watanabe T (1997) Light-induced amphiphilic surfaces. Nature 388:431–432View ArticleGoogle Scholar
- Hupa L, Piispanen M (2011) Comparison of self-cleaning properties of three titania coatings on float glass. Appl Surf Sci 258:1126–1131View ArticleGoogle Scholar
- Fujishima A, Liu Z, Zhang X, Murakami T (2008) Sol–gel SiO2/TiO2 bilayer films with self-cleaning and antireflection properties. Solar Energy Mater Solar Cells 92:1434–1438View ArticleGoogle Scholar
- Houmard M, Riassetto D, Roussel F, Bourgeois A, Berthomé G, Joud JC, Langlet M (2007) Morphology and natural wettability properties of sol–gel derived TiO2–SiO2 composite thin films. Appl Surf Sci 254:1405–1414View ArticleGoogle Scholar
- Sarver T, Al-Qaraghuli A, Kazmerski LL (2013) A comprehensive review of the impact of dust on the use of solar energy:History, investigations, results, literature, and mitigation approaches. Renew Sustain Energy Rev 22:698–733View ArticleGoogle Scholar
- Ghazi S, SayighA KLP (2014) Dust effect on flat surfaces–A review paper. Renew Sustain Energy Rev 33:742–751View ArticleGoogle Scholar
- Quan X, Su Y, Chen S, Zhao H, Su YZY, Chen S, Zhang Y (2008) A silicon-doped TiO2 nanotube arrays electrode with enhanced photoelectro catalytic activity. Appl Surf Sci 255:2167–2172View ArticleGoogle Scholar
- Lee K, Lee SH (2007) Influence of SiO2 interlayer on the hydrophilicity of TiO2/SiO2/glass produced by RF-magnetron sputtering. Mater Lett 61:3516–3518View ArticleGoogle Scholar
- Kikuchi N, Tonooka K (2013) Super-hydrophilic and solar-heat-reflective coatings for smart windows. Thin Solid Films 532:147–150View ArticleGoogle Scholar
- Sanjabi S, Nejand BA, Ahmadi V (2010) The effect of sputtering gas pressure on structure and photocatalytic properties of nanostructured titanium oxide self-cleaning thin film. Vacuum 85:400–405View ArticleGoogle Scholar
- Eiamchai P, Chindaudom P, Horprathum M, Patthanasettakul V, Limsuwan P (2009) Design and investigation of photo-induced super-hydrophilic materials for car mirrors. Materials Design 30:3428–3435View ArticleGoogle Scholar
- Çamurlu HE, Kesmez O, Burunkaya E, Arpaç E (2009) Sol–gel preparation and characterization of anti-reflective and self-cleaning SiO2–TiO2 double-layer nanometric films. Solar Energy Mater Solar Cells 93:1833–1839View ArticleGoogle Scholar
- Zhao JX, Li A, Jin Y, MuggliD PDT, Aranwela H, Marasinghe GK, Knutson T, Brockman G (2013) Nanoscale effects of silica particle supports on the formation and properties of TiO2 nanocatalysts. Nanoscale 5:5854–5862View ArticleGoogle Scholar
- Kermadi S, Agoudjil N, Sali S, Boumaour M, Bourgeois S, Marco de Lucas MC (2014) Sol–gel synthesis of xTiO2(100 – X)SiO2nanocomposite thin films: structure, optical and antireflection properties. Thin Solid Films 564:170–178View ArticleGoogle Scholar
- Luo C, Chuang L, Yang S (2011) The structure and mechanical properties of thick rutile-TiO2 films using different coatings treatments. Appl Surf Sci 258:297–303View ArticleGoogle Scholar
This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.